#------------------------------------------------------------------------------
#$Date: 2016-03-21 01:21:50 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178377 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/19/4001925.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4001925
loop_
_publ_author_name
'Forbes, Scott'
'Yuan, Fang'
'Saparov, Bayrammurad'
'Sefat, Athena S.'
'Kosuda, Kosuke'
'Kolodiazhnyi, Taras'
'Mozharivskyj, Yurij'
_publ_section_title
;
 Synthesis, Crystal Structure, and Electronic Properties of the
 CaRE3SbO4and Ca2RE8Sb3O10phases (RE = Rare-Earth Metal)
;
_journal_issue                   7
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2289
_journal_paper_doi               10.1021/cm500157y
_journal_volume                  26
_journal_year                    2014
_chemical_formula_sum            'Ca2.04 O10 Pr7.96 Sb2.97'
_chemical_formula_weight         1724.90
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 93.54(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   13.651(3)
_cell_length_b                   3.9229(8)
_cell_length_c                   17.628(4)
_cell_measurement_reflns_used    5330
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      34.84
_cell_measurement_theta_min      2.99
_cell_volume                     942.2(4)
_computing_cell_refinement       X-Area
_computing_data_collection       X-Area
_computing_data_reduction        X-Red32
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.951
_diffrn_measured_fraction_theta_max 0.951
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0496
_diffrn_reflns_av_sigmaI/netI    0.0856
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            5330
_diffrn_reflns_theta_full        34.55
_diffrn_reflns_theta_max         34.55
_diffrn_reflns_theta_min         2.99
_exptl_absorpt_coefficient_mu    24.913
_exptl_absorpt_correction_T_max  0.3845
_exptl_absorpt_correction_T_min  0.3046
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   X-Red
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    6.080
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Block
_exptl_crystal_F_000             1483.7
_exptl_crystal_size_max          0.0709
_exptl_crystal_size_mid          0.0590
_exptl_crystal_size_min          0.0546
_refine_diff_density_max         2.291
_refine_diff_density_min         -2.047
_refine_diff_density_rms         0.364
_refine_ls_extinction_coef       0.000465(13)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.802
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     91
_refine_ls_number_reflns         2146
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.802
_refine_ls_R_factor_all          0.0881
_refine_ls_R_factor_gt           0.0356
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0064P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0339
_refine_ls_wR_factor_ref         0.0395
_reflns_number_gt                1265
_reflns_number_total             2146
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm500157y_si_004.cif
_cod_data_source_block           c2m
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Numerical'
changed to 'numerical' according to
/usr/data/users/saulius/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for
 ./tmp-cod-update-bibliographies-15567/cifs/4001925.cif.
;
_cod_original_cell_volume        942.2(3)
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               4001925
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ca1 Ca 0.8142(12) 0.0000 0.0797(7) 0.0107(3) Uani 0.331(7) 2 d SP
Pr1 Pr 0.82717(12) 0.0000 0.06432(8) 0.0107(3) Uani 0.669(7) 2 d SP
Ca2 Ca 0.1224(11) 0.0000 0.1517(8) 0.0117(3) Uani 0.276(8) 2 d SP
Pr2 Pr 0.09421(10) 0.0000 0.13618(7) 0.0117(3) Uani 0.724(8) 2 d SP
Ca3 Ca 0.4179(13) 0.0000 0.2351(11) 0.0132(3) Uani 0.231(7) 2 d SP
Pr3 Pr 0.43739(9) 0.0000 0.25062(8) 0.0132(3) Uani 0.769(7) 2 d SP
Ca4 Ca 0.265(2) 0.0000 0.6925(17) 0.0111(2) Uani 0.120(7) 2 d SP
Pr4 Pr 0.29385(7) 0.0000 0.68150(4) 0.0111(2) Uani 0.880(7) 2 d SP
Ca5 Ca 0.364(3) 0.0000 0.495(3) 0.0113(2) Uani 0.059(7) 2 d SP
Pr5 Pr 0.35313(5) 0.0000 0.46466(6) 0.0113(2) Uani 0.941(7) 2 d SP
Sb1 Sb 0.0000 0.5000 0.0000 0.0195(3) Uani 1 4 d S
Sb2 Sb 0.03143(7) 0.036(2) 0.38820(6) 0.0240(11) Uani 0.491(4) 1 d P
O1 O 0.2356(6) 0.0000 0.0691(4) 0.0166(15) Uani 1 2 d S
O2 O 0.6060(5) 0.0000 0.2062(3) 0.0159(14) Uani 1 2 d S
O3 O 0.0772(6) 0.0000 0.8215(4) 0.0187(15) Uani 1 2 d S
O4 O 0.2959(6) 0.0000 0.3154(5) 0.0278(18) Uani 1 2 d S
O5 O 0.2326(5) 0.0000 0.5566(3) 0.0126(13) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pr Pr -0.2180 2.8214 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Ca1 O1 111.1(4) 5_656 3_545
O3 Ca1 O1 111.1(4) 5_656 3
O1 Ca1 O1 122.5(8) 3_545 3
O3 Ca1 O1 152.8(7) 5_656 5_655
O1 Ca1 O1 80.0(4) 3_545 5_655
O1 Ca1 O1 80.0(4) 3 5_655
O3 Ca1 Sb1 81.5(4) 5_656 1_655
O1 Ca1 Sb1 143.0(5) 3_545 1_655
O1 Ca1 Sb1 80.4(3) 3 1_655
O1 Ca1 Sb1 75.9(3) 5_655 1_655
O3 Ca1 Sb1 81.5(4) 5_656 1_645
O1 Ca1 Sb1 80.4(3) 3_545 1_645
O1 Ca1 Sb1 143.0(5) 3 1_645
O1 Ca1 Sb1 75.9(3) 5_655 1_645
Sb1 Ca1 Sb1 66.8(3) 1_655 1_645
O3 Ca1 Ca2 101.0(5) 5_656 3_545
O1 Ca1 Ca2 35.8(3) 3_545 3_545
O1 Ca1 Ca2 98.8(6) 3 3_545
O1 Ca1 Ca2 101.6(5) 5_655 3_545
Sb1 Ca1 Ca2 177.5(6) 1_655 3_545
Sb1 Ca1 Ca2 113.19(13) 1_645 3_545
O3 Ca1 Ca2 101.0(5) 5_656 3
O1 Ca1 Ca2 98.8(6) 3_545 3
O1 Ca1 Ca2 35.8(3) 3 3
O1 Ca1 Ca2 101.6(5) 5_655 3
Sb1 Ca1 Ca2 113.19(13) 1_655 3
Sb1 Ca1 Ca2 177.5(6) 1_645 3
Ca2 Ca1 Ca2 66.7(4) 3_545 3
O3 Ca1 Ca3 35.6(2) 5_656 3
O1 Ca1 Ca3 135.0(6) 3_545 3
O1 Ca1 Ca3 75.5(3) 3 3
O1 Ca1 Ca3 144.6(3) 5_655 3
Sb1 Ca1 Ca3 75.1(3) 1_655 3
Sb1 Ca1 Ca3 110.2(5) 1_645 3
Ca2 Ca1 Ca3 107.0(5) 3_545 3
Ca2 Ca1 Ca3 72.0(4) 3 3
O3 Ca1 Ca3 35.6(2) 5_656 3_545
O1 Ca1 Ca3 75.5(3) 3_545 3_545
O1 Ca1 Ca3 135.0(6) 3 3_545
O1 Ca1 Ca3 144.6(3) 5_655 3_545
Sb1 Ca1 Ca3 110.2(5) 1_655 3_545
Sb1 Ca1 Ca3 75.1(3) 1_645 3_545
Ca2 Ca1 Ca3 72.0(4) 3_545 3_545
Ca2 Ca1 Ca3 107.0(5) 3 3_545
Ca3 Ca1 Ca3 66.3(4) 3 3_545
O3 Ca1 Pr1 147.46(14) 5_656 7_645
O1 Ca1 Pr1 40.8(3) 3_545 7_645
O1 Ca1 Pr1 100.5(5) 3 7_645
O1 Ca1 Pr1 39.39(19) 5_655 7_645
Sb1 Ca1 Pr1 112.3(3) 1_655 7_645
Sb1 Ca1 Pr1 77.82(18) 1_645 7_645
Ca2 Ca1 Pr1 65.5(3) 3_545 7_645
Ca2 Ca1 Pr1 100.0(5) 3 7_645
Ca3 Ca1 Pr1 171.2(5) 3 7_645
Ca3 Ca1 Pr1 113.74(17) 3_545 7_645
O3 Ca1 Pr1 147.46(14) 5_656 7_655
O1 Ca1 Pr1 100.5(5) 3_545 7_655
O1 Ca1 Pr1 40.8(3) 3 7_655
O1 Ca1 Pr1 39.39(19) 5_655 7_655
Sb1 Ca1 Pr1 77.82(18) 1_655 7_655
Sb1 Ca1 Pr1 112.3(3) 1_645 7_655
Ca2 Ca1 Pr1 100.0(5) 3_545 7_655
Ca2 Ca1 Pr1 65.5(3) 3 7_655
Ca3 Ca1 Pr1 113.74(17) 3 7_655
Ca3 Ca1 Pr1 171.2(5) 3_545 7_655
Pr1 Ca1 Pr1 64.8(2) 7_645 7_655
O1 Pr1 O1 114.7(3) 3_545 3
O1 Pr1 O3 103.98(19) 3_545 5_656
O1 Pr1 O3 103.98(19) 3 5_656
O1 Pr1 O1 83.0(2) 3_545 5_655
O1 Pr1 O1 83.0(2) 3 5_655
O3 Pr1 O1 166.4(3) 5_656 5_655
O1 Pr1 Sb1 154.62(16) 3_545 1_655
O1 Pr1 Sb1 84.78(16) 3 1_655
O3 Pr1 Sb1 85.59(16) 5_656 1_655
O1 Pr1 Sb1 83.46(15) 5_655 1_655
O1 Pr1 Sb1 84.78(16) 3_545 1_645
O1 Pr1 Sb1 154.62(16) 3 1_645
O3 Pr1 Sb1 85.59(16) 5_656 1_645
O1 Pr1 Sb1 83.46(15) 5_655 1_645
Sb1 Pr1 Sb1 72.40(4) 1_655 1_645
O1 Pr1 Pr1 42.82(17) 3_545 7_645
O1 Pr1 Pr1 100.85(18) 3 7_645
O3 Pr1 Pr1 145.36(6) 5_656 7_645
O1 Pr1 Pr1 40.20(10) 5_655 7_645
Sb1 Pr1 Pr1 120.63(6) 1_655 7_645
Sb1 Pr1 Pr1 82.12(4) 1_645 7_645
O1 Pr1 Pr1 100.85(18) 3_545 7_655
O1 Pr1 Pr1 42.82(17) 3 7_655
O3 Pr1 Pr1 145.36(6) 5_656 7_655
O1 Pr1 Pr1 40.20(10) 5_655 7_655
Sb1 Pr1 Pr1 82.12(4) 1_655 7_655
Sb1 Pr1 Pr1 120.63(6) 1_645 7_655
Pr1 Pr1 Pr1 66.38(6) 7_645 7_655
O1 Pr1 Ca1 46.7(2) 3_545 7_645
O1 Pr1 Ca1 102.4(2) 3 7_645
O3 Pr1 Ca1 147.34(12) 5_656 7_645
O1 Pr1 Ca1 36.61(15) 5_655 7_645
Sb1 Pr1 Ca1 115.8(2) 1_655 7_645
Sb1 Pr1 Ca1 78.6(2) 1_645 7_645
Pr1 Pr1 Ca1 5.1(2) 7_645 7_645
Pr1 Pr1 Ca1 65.82(10) 7_655 7_645
O1 Pr1 Ca1 102.4(2) 3_545 7_655
O1 Pr1 Ca1 46.7(2) 3 7_655
O3 Pr1 Ca1 147.34(12) 5_656 7_655
O1 Pr1 Ca1 36.61(15) 5_655 7_655
Sb1 Pr1 Ca1 78.6(2) 1_655 7_655
Sb1 Pr1 Ca1 115.8(2) 1_645 7_655
Pr1 Pr1 Ca1 65.82(10) 7_645 7_655
Pr1 Pr1 Ca1 5.1(2) 7_655 7_655
Ca1 Pr1 Ca1 64.8(2) 7_645 7_655
O1 Pr1 Ca3 124.3(3) 3_545 3
O1 Pr1 Ca3 71.4(3) 3 3
O3 Pr1 Ca3 33.35(17) 5_656 3
O1 Pr1 Ca3 148.28(15) 5_655 3
Sb1 Pr1 Ca3 76.0(3) 1_655 3
Sb1 Pr1 Ca3 112.2(3) 1_645 3
Pr1 Pr1 Ca3 161.6(3) 7_645 3
Pr1 Pr1 Ca3 112.02(16) 7_655 3
Ca1 Pr1 Ca3 166.7(4) 7_645 3
Ca1 Pr1 Ca3 114.29(19) 7_655 3
O1 Pr1 Ca3 71.4(3) 3_545 3_545
O1 Pr1 Ca3 124.3(3) 3 3_545
O3 Pr1 Ca3 33.35(17) 5_656 3_545
O1 Pr1 Ca3 148.28(15) 5_655 3_545
Sb1 Pr1 Ca3 112.2(3) 1_655 3_545
Sb1 Pr1 Ca3 76.0(3) 1_645 3_545
Pr1 Pr1 Ca3 112.02(16) 7_645 3_545
Pr1 Pr1 Ca3 161.6(3) 7_655 3_545
Ca1 Pr1 Ca3 114.29(19) 7_645 3_545
Ca1 Pr1 Ca3 166.7(4) 7_655 3_545
Ca3 Pr1 Ca3 63.3(3) 3 3_545
O1 Ca2 O2 112.6(4) . 3_455
O1 Ca2 O2 112.6(4) . 3_445
O2 Ca2 O2 126.1(7) 3_455 3_445
O1 Ca2 O3 148.1(8) . 5_556
O2 Ca2 O3 78.5(4) 3_455 5_556
O2 Ca2 O3 78.5(4) 3_445 5_556
O1 Ca2 Ca1 36.8(2) . 3_455
O2 Ca2 Ca1 76.2(3) 3_455 3_455
O2 Ca2 Ca1 137.9(6) 3_445 3_455
O3 Ca2 Ca1 143.6(3) 5_556 3_455
O1 Ca2 Ca1 36.8(2) . 3_445
O2 Ca2 Ca1 137.9(6) 3_455 3_445
O2 Ca2 Ca1 76.2(3) 3_445 3_445
O3 Ca2 Ca1 143.6(3) 5_556 3_445
Ca1 Ca2 Ca1 66.7(4) 3_455 3_445
O1 Ca2 Ca4 102.7(7) . 7_556
O2 Ca2 Ca4 40.5(4) 3_455 7_556
O2 Ca2 Ca4 101.6(6) 3_445 7_556
O3 Ca2 Ca4 104.0(6) 5_556 7_556
Ca1 Ca2 Ca4 71.8(6) 3_455 7_556
Ca1 Ca2 Ca4 106.3(7) 3_445 7_556
O1 Ca2 Ca4 102.7(7) . 7_546
O2 Ca2 Ca4 101.6(6) 3_455 7_546
O2 Ca2 Ca4 40.5(4) 3_445 7_546
O3 Ca2 Ca4 104.0(6) 5_556 7_546
Ca1 Ca2 Ca4 106.3(7) 3_455 7_546
Ca1 Ca2 Ca4 71.8(6) 3_445 7_546
Ca4 Ca2 Ca4 65.3(5) 7_556 7_546
O1 Ca2 Sb1 79.7(4) . 1_545
O2 Ca2 Sb1 138.3(6) 3_455 1_545
O2 Ca2 Sb1 77.6(3) 3_445 1_545
O3 Ca2 Sb1 73.5(3) 5_556 1_545
Ca1 Ca2 Sb1 110.4(4) 3_455 1_545
Ca1 Ca2 Sb1 75.9(3) 3_445 1_545
Ca4 Ca2 Sb1 177.5(7) 7_556 1_545
Ca4 Ca2 Sb1 114.7(2) 7_546 1_545
O1 Ca2 Sb1 79.7(4) . .
O2 Ca2 Sb1 77.6(3) 3_455 .
O2 Ca2 Sb1 138.3(6) 3_445 .
O3 Ca2 Sb1 73.5(3) 5_556 .
Ca1 Ca2 Sb1 75.9(3) 3_455 .
Ca1 Ca2 Sb1 110.4(4) 3_445 .
Ca4 Ca2 Sb1 114.7(2) 7_556 .
Ca4 Ca2 Sb1 177.5(7) 7_546 .
Sb1 Ca2 Sb1 65.2(3) 1_545 .
O1 Ca2 Pr4 109.6(5) . 7_556
O2 Ca2 Pr4 37.5(3) 3_455 7_556
O2 Ca2 Pr4 99.4(5) 3_445 7_556
O3 Ca2 Pr4 97.1(3) 5_556 7_556
Ca1 Ca2 Pr4 77.9(3) 3_455 7_556
Ca1 Ca2 Pr4 112.4(5) 3_445 7_556
Ca4 Ca2 Pr4 7.0(5) 7_556 7_556
Ca4 Ca2 Pr4 65.5(4) 7_546 7_556
Sb1 Ca2 Pr4 170.5(4) 1_545 7_556
Sb1 Ca2 Pr4 114.09(6) . 7_556
O1 Ca2 Pr4 109.6(5) . 7_546
O2 Ca2 Pr4 99.4(5) 3_455 7_546
O2 Ca2 Pr4 37.5(3) 3_445 7_546
O3 Ca2 Pr4 97.1(3) 5_556 7_546
Ca1 Ca2 Pr4 112.4(5) 3_455 7_546
Ca1 Ca2 Pr4 77.9(3) 3_445 7_546
Ca4 Ca2 Pr4 65.5(4) 7_556 7_546
Ca4 Ca2 Pr4 7.0(5) 7_546 7_546
Sb1 Ca2 Pr4 114.09(6) 1_545 7_546
Sb1 Ca2 Pr4 170.5(4) . 7_546
Pr4 Ca2 Pr4 64.9(3) 7_556 7_546
O2 Pr2 O2 115.6(3) 3_455 3_445
O2 Pr2 O1 103.8(2) 3_455 .
O2 Pr2 O1 103.8(2) 3_445 .
O2 Pr2 O3 82.90(19) 3_455 5_556
O2 Pr2 O3 82.90(19) 3_445 5_556
O1 Pr2 O3 166.9(2) . 5_556
O2 Pr2 Sb1 154.39(16) 3_455 1_545
O2 Pr2 Sb1 83.98(13) 3_445 1_545
O1 Pr2 Sb1 85.91(15) . 1_545
O3 Pr2 Sb1 83.53(13) 5_556 1_545
O2 Pr2 Sb1 83.98(13) 3_455 .
O2 Pr2 Sb1 154.39(16) 3_445 .
O1 Pr2 Sb1 85.91(15) . .
O3 Pr2 Sb1 83.53(13) 5_556 .
Sb1 Pr2 Sb1 72.97(4) 1_545 .
O2 Pr2 Pr3 100.74(16) 3_455 3_445
O2 Pr2 Pr3 42.83(18) 3_445 3_445
O1 Pr2 Pr3 145.46(6) . 3_445
O3 Pr2 Pr3 40.07(8) 5_556 3_445
Sb1 Pr2 Pr3 82.28(3) 1_545 3_445
Sb1 Pr2 Pr3 120.78(4) . 3_445
O2 Pr2 Pr3 42.83(18) 3_455 3_455
O2 Pr2 Pr3 100.74(16) 3_445 3_455
O1 Pr2 Pr3 145.46(6) . 3_455
O3 Pr2 Pr3 40.07(8) 5_556 3_455
Sb1 Pr2 Pr3 120.78(4) 1_545 3_455
Sb1 Pr2 Pr3 82.28(3) . 3_455
Pr3 Pr2 Pr3 65.82(3) 3_445 3_455
O2 Pr2 Ca3 103.2(3) 3_455 3_445
O2 Pr2 Ca3 46.7(3) 3_445 3_445
O1 Pr2 Ca3 147.09(17) . 3_445
O3 Pr2 Ca3 36.5(2) 5_556 3_445
Sb1 Pr2 Ca3 77.8(2) 1_545 3_445
Sb1 Pr2 Ca3 115.5(2) . 3_445
Pr3 Pr2 Ca3 5.8(3) 3_445 3_445
Pr3 Pr2 Ca3 65.90(16) 3_455 3_445
O2 Pr2 Ca3 46.7(3) 3_455 3_455
O2 Pr2 Ca3 103.2(3) 3_445 3_455
O1 Pr2 Ca3 147.09(17) . 3_455
O3 Pr2 Ca3 36.5(2) 5_556 3_455
Sb1 Pr2 Ca3 115.5(2) 1_545 3_455
Sb1 Pr2 Ca3 77.8(2) . 3_455
Pr3 Pr2 Ca3 65.90(16) 3_445 3_455
Pr3 Pr2 Ca3 5.8(3) 3_455 3_455
Ca3 Pr2 Ca3 65.3(3) 3_445 3_455
O2 Pr2 Pr1 119.10(15) 3_455 5_655
O2 Pr2 Pr1 119.10(15) 3_445 5_655
O1 Pr2 Pr1 39.40(18) . 5_655
O3 Pr2 Pr1 127.46(16) 5_556 5_655
Sb1 Pr2 Pr1 55.70(3) 1_545 5_655
Sb1 Pr2 Pr1 55.70(3) . 5_655
Pr3 Pr2 Pr1 137.69(4) 3_445 5_655
Pr3 Pr2 Pr1 137.69(4) 3_455 5_655
Ca3 Pr2 Pr1 133.5(2) 3_445 5_655
Ca3 Pr2 Pr1 133.5(2) 3_455 5_655
O2 Pr2 Ca1 70.7(2) 3_455 3_455
O2 Pr2 Ca1 123.4(3) 3_445 3_455
O1 Pr2 Ca1 33.51(13) . 3_455
O3 Pr2 Ca1 148.66(12) 5_556 3_455
Sb1 Pr2 Ca1 113.46(17) 1_545 3_455
Sb1 Pr2 Ca1 77.3(2) . 3_455
Pr3 Pr2 Ca1 159.9(2) 3_445 3_455
Pr3 Pr2 Ca1 111.97(11) 3_455 3_455
Ca3 Pr2 Ca1 165.8(3) 3_445 3_455
Ca3 Pr2 Ca1 114.1(2) 3_455 3_455
Pr1 Pr2 Ca1 58.22(17) 5_655 3_455
O3 Ca3 O3 125.8(9) 7_546 7_556
O3 Ca3 O4 109.2(5) 7_546 .
O3 Ca3 O4 109.2(5) 7_556 .
O3 Ca3 O2 81.7(6) 7_546 .
O3 Ca3 O2 81.7(6) 7_556 .
O4 Ca3 O2 152.2(9) . .
O3 Ca3 Ca4 73.0(5) 7_546 7_546
O3 Ca3 Ca4 135.3(8) 7_556 7_546
O4 Ca3 Ca4 36.3(4) . 7_546
O2 Ca3 Ca4 142.9(4) . 7_546
O3 Ca3 Ca4 135.3(8) 7_546 7_556
O3 Ca3 Ca4 73.0(5) 7_556 7_556
O4 Ca3 Ca4 36.3(4) . 7_556
O2 Ca3 Ca4 142.9(4) . 7_556
Ca4 Ca3 Ca4 68.6(7) 7_546 7_556
O3 Ca3 Sb2 141.3(6) 7_546 8
O3 Ca3 Sb2 82.1(3) 7_556 8
O4 Ca3 Sb2 80.0(5) . 8
O2 Ca3 Sb2 76.3(4) . 8
Ca4 Ca3 Sb2 107.5(7) 7_546 8
Ca4 Ca3 Sb2 73.8(5) 7_556 8
O3 Ca3 Sb2 82.1(3) 7_546 3_545
O3 Ca3 Sb2 141.3(6) 7_556 3_545
O4 Ca3 Sb2 80.0(5) . 3_545
O2 Ca3 Sb2 76.3(4) . 3_545
Ca4 Ca3 Sb2 73.8(5) 7_546 3_545
Ca4 Ca3 Sb2 107.5(7) 7_556 3_545
Sb2 Ca3 Sb2 62.0(4) 8 3_545
O3 Ca3 Ca1 35.8(4) 7_546 3_445
O3 Ca3 Ca1 99.4(6) 7_556 3_445
O4 Ca3 Ca1 102.0(6) . 3_445
O2 Ca3 Ca1 101.2(6) . 3_445
Ca4 Ca3 Ca1 73.4(5) 7_546 3_445
Ca4 Ca3 Ca1 109.2(6) 7_556 3_445
Sb2 Ca3 Ca1 176.9(5) 8 3_445
Sb2 Ca3 Ca1 115.81(17) 3_545 3_445
O3 Ca3 Ca1 99.4(6) 7_546 3_455
O3 Ca3 Ca1 35.8(4) 7_556 3_455
O4 Ca3 Ca1 102.0(6) . 3_455
O2 Ca3 Ca1 101.2(6) . 3_455
Ca4 Ca3 Ca1 109.2(6) 7_546 3_455
Ca4 Ca3 Ca1 73.4(5) 7_556 3_455
Sb2 Ca3 Ca1 115.81(17) 8 3_455
Sb2 Ca3 Ca1 176.9(5) 3_545 3_455
Ca1 Ca3 Ca1 66.3(4) 3_445 3_455
O3 Ca3 Pr2 102.9(7) 7_546 3
O3 Ca3 Pr2 42.5(4) 7_556 3
O4 Ca3 Pr2 147.09(19) . 3
O2 Ca3 Pr2 39.5(2) . 3
Ca4 Ca3 Pr2 172.8(8) 7_546 3
Ca4 Ca3 Pr2 112.6(3) 7_556 3
Sb2 Ca3 Pr2 79.4(3) 8 3
Sb2 Ca3 Pr2 111.8(5) 3_545 3
Ca1 Ca3 Pr2 99.8(5) 3_445 3
Ca1 Ca3 Pr2 65.2(3) 3_455 3
O3 Ca3 Pr2 42.5(4) 7_546 3_545
O3 Ca3 Pr2 102.9(7) 7_556 3_545
O4 Ca3 Pr2 147.09(19) . 3_545
O2 Ca3 Pr2 39.5(2) . 3_545
Ca4 Ca3 Pr2 112.6(3) 7_546 3_545
Ca4 Ca3 Pr2 172.8(8) 7_556 3_545
Sb2 Ca3 Pr2 111.8(5) 8 3_545
Sb2 Ca3 Pr2 79.4(3) 3_545 3_545
Ca1 Ca3 Pr2 65.2(3) 3_445 3_545
Ca1 Ca3 Pr2 99.8(5) 3_455 3_545
Pr2 Ca3 Pr2 65.3(3) 3 3_545
O4 Pr3 O3 102.9(2) . 7_546
O4 Pr3 O3 102.9(2) . 7_556
O3 Pr3 O3 114.0(3) 7_546 7_556
O4 Pr3 O2 168.7(3) . .
O3 Pr3 O2 83.0(2) 7_546 .
O3 Pr3 O2 83.0(2) 7_556 .
O4 Pr3 Sb2 86.23(19) . 8
O3 Pr3 Sb2 153.62(19) 7_546 8
O3 Pr3 Sb2 87.26(18) 7_556 8
O2 Pr3 Sb2 84.48(12) . 8
O4 Pr3 Sb2 86.23(19) . 3_545
O3 Pr3 Sb2 87.26(18) 7_546 3_545
O3 Pr3 Sb2 153.6(2) 7_556 3_545
O2 Pr3 Sb2 84.48(12) . 3_545
Sb2 Pr3 Sb2 68.5(2) 8 3_545
O4 Pr3 Sb2 86.42(19) . 3
O3 Pr3 Sb2 157.18(19) 7_546 3
O3 Pr3 Sb2 83.36(17) 7_556 3
O2 Pr3 Sb2 84.75(12) . 3
Sb2 Pr3 Sb2 4.0(2) 8 3
Sb2 Pr3 Sb2 72.44(4) 3_545 3
O4 Pr3 Sb2 86.42(18) . 8_545
O3 Pr3 Sb2 83.36(17) 7_546 8_545
O3 Pr3 Sb2 157.18(19) 7_556 8_545
O2 Pr3 Sb2 84.75(12) . 8_545
Sb2 Pr3 Sb2 72.44(4) 8 8_545
Sb2 Pr3 Sb2 4.0(2) 3_545 8_545
Sb2 Pr3 Sb2 76.4(2) 3 8_545
O4 Pr3 Ca4 34.5(3) . 7_546
O3 Pr3 Ca4 69.6(4) 7_546 7_546
O3 Pr3 Ca4 124.7(4) 7_556 7_546
O2 Pr3 Ca4 146.8(3) . 7_546
Sb2 Pr3 Ca4 112.1(4) 8 7_546
Sb2 Pr3 Ca4 76.1(4) 3_545 7_546
Sb2 Pr3 Ca4 113.7(4) 3 7_546
Sb2 Pr3 Ca4 74.1(4) 8_545 7_546
O4 Pr3 Ca4 34.5(3) . 7_556
O3 Pr3 Ca4 124.7(4) 7_546 7_556
O3 Pr3 Ca4 69.6(4) 7_556 7_556
O2 Pr3 Ca4 146.8(3) . 7_556
Sb2 Pr3 Ca4 76.1(4) 8 7_556
Sb2 Pr3 Ca4 112.1(4) 3_545 7_556
Sb2 Pr3 Ca4 74.1(4) 3 7_556
Sb2 Pr3 Ca4 113.7(4) 8_545 7_556
Ca4 Pr3 Ca4 66.3(6) 7_546 7_556
O4 Pr3 Pr2 145.21(7) . 3
O3 Pr3 Pr2 100.69(17) 7_546 3
O3 Pr3 Pr2 43.47(19) 7_556 3
O2 Pr3 Pr2 39.51(8) . 3
Sb2 Pr3 Pr2 83.79(8) 8 3
Sb2 Pr3 Pr2 120.21(6) 3_545 3
Sb2 Pr3 Pr2 81.47(7) 3 3
Sb2 Pr3 Pr2 121.58(5) 8_545 3
Ca4 Pr3 Pr2 161.5(4) 7_546 3
Ca4 Pr3 Pr2 110.7(3) 7_556 3
O4 Pr3 Pr2 145.21(7) . 3_545
O3 Pr3 Pr2 43.47(19) 7_546 3_545
O3 Pr3 Pr2 100.69(17) 7_556 3_545
O2 Pr3 Pr2 39.51(8) . 3_545
Sb2 Pr3 Pr2 120.21(6) 8 3_545
Sb2 Pr3 Pr2 83.79(7) 3_545 3_545
Sb2 Pr3 Pr2 121.58(5) 3 3_545
Sb2 Pr3 Pr2 81.47(7) 8_545 3_545
Ca4 Pr3 Pr2 110.7(3) 7_546 3_545
Ca4 Pr3 Pr2 161.5(4) 7_556 3_545
Pr2 Pr3 Pr2 65.82(3) 3 3_545
O4 Ca4 O4 133.7(15) 7_546 7_556
O4 Ca4 O5 83.5(8) 7_546 .
O4 Ca4 O5 83.5(8) 7_556 .
O4 Ca4 O2 108.1(7) 7_546 5_656
O4 Ca4 O2 108.1(7) 7_556 5_656
O5 Ca4 O2 144.4(15) . 5_656
O4 Ca4 Ca3 38.6(6) 7_546 7_546
O4 Ca4 Ca3 104.8(12) 7_556 7_546
O5 Ca4 Ca3 105.7(9) . 7_546
O2 Ca4 Ca3 103.5(9) 5_656 7_546
O4 Ca4 Ca3 104.8(12) 7_546 7_556
O4 Ca4 Ca3 38.6(6) 7_556 7_556
O5 Ca4 Ca3 105.7(9) . 7_556
O2 Ca4 Ca3 103.5(9) 5_656 7_556
Ca3 Ca4 Ca3 68.6(7) 7_546 7_556
O4 Ca4 Pr3 37.7(6) 7_546 7_546
O4 Ca4 Pr3 102.4(11) 7_556 7_546
O5 Ca4 Pr3 100.3(8) . 7_546
O2 Ca4 Pr3 109.3(9) 5_656 7_546
Ca3 Ca4 Pr3 5.8(3) 7_546 7_546
Ca3 Ca4 Pr3 67.8(6) 7_556 7_546
O4 Ca4 Pr3 102.4(11) 7_546 7_556
O4 Ca4 Pr3 37.7(6) 7_556 7_556
O5 Ca4 Pr3 100.3(8) . 7_556
O2 Ca4 Pr3 109.3(9) 5_656 7_556
Ca3 Ca4 Pr3 67.8(6) 7_546 7_556
Ca3 Ca4 Pr3 5.8(3) 7_556 7_556
Pr3 Ca4 Pr3 66.3(6) 7_546 7_556
O4 Ca4 Ca2 133.7(11) 7_546 7_556
O4 Ca4 Ca2 72.5(6) 7_556 7_556
O5 Ca4 Ca2 142.6(7) . 7_556
O2 Ca4 Ca2 36.1(3) 5_656 7_556
Ca3 Ca4 Ca2 107.8(9) 7_546 7_556
Ca3 Ca4 Ca2 72.4(5) 7_556 7_556
Pr3 Ca4 Ca2 112.4(9) 7_546 7_556
Pr3 Ca4 Ca2 77.9(5) 7_556 7_556
O4 Ca4 Ca2 72.5(6) 7_546 7_546
O4 Ca4 Ca2 133.7(11) 7_556 7_546
O5 Ca4 Ca2 142.6(7) . 7_546
O2 Ca4 Ca2 36.1(3) 5_656 7_546
Ca3 Ca4 Ca2 72.4(5) 7_546 7_546
Ca3 Ca4 Ca2 107.8(9) 7_556 7_546
Pr3 Ca4 Ca2 77.9(5) 7_546 7_546
Pr3 Ca4 Ca2 112.4(9) 7_556 7_546
Ca2 Ca4 Ca2 65.3(5) 7_556 7_546
O4 Ca4 Sb2 137.0(12) 7_546 7_556
O4 Ca4 Sb2 79.7(7) 7_556 7_556
O5 Ca4 Sb2 73.3(8) . 7_556
O2 Ca4 Sb2 75.8(7) 5_656 7_556
Ca3 Ca4 Sb2 175.4(6) 7_546 7_556
Ca3 Ca4 Sb2 116.1(2) 7_556 7_556
Pr3 Ca4 Sb2 173.1(8) 7_546 7_556
Pr3 Ca4 Sb2 116.84(14) 7_556 7_556
Ca2 Ca4 Sb2 74.5(4) 7_556 7_556
Ca2 Ca4 Sb2 105.4(7) 7_546 7_556
O4 Ca4 Sb2 79.7(7) 7_546 4_546
O4 Ca4 Sb2 137.0(12) 7_556 4_546
O5 Ca4 Sb2 73.3(8) . 4_546
O2 Ca4 Sb2 75.8(7) 5_656 4_546
Ca3 Ca4 Sb2 116.1(2) 7_546 4_546
Ca3 Ca4 Sb2 175.4(6) 7_556 4_546
Pr3 Ca4 Sb2 116.84(14) 7_546 4_546
Pr3 Ca4 Sb2 173.1(8) 7_556 4_546
Ca2 Ca4 Sb2 105.4(7) 7_556 4_546
Ca2 Ca4 Sb2 74.5(4) 7_546 4_546
Sb2 Ca4 Sb2 59.3(6) 7_556 4_546
O5 Pr4 O4 82.0(2) . 7_546
O5 Pr4 O4 82.0(2) . 7_556
O4 Pr4 O4 115.8(4) 7_546 7_556
O5 Pr4 O2 165.5(2) . 5_656
O4 Pr4 O2 105.3(2) 7_546 5_656
O4 Pr4 O2 105.3(2) 7_556 5_656
O5 Pr4 Sb2 82.65(14) . 7_556
O4 Pr4 Sb2 150.7(2) 7_546 7_556
O4 Pr4 Sb2 86.4(2) 7_556 7_556
O2 Pr4 Sb2 85.23(15) 5_656 7_556
O5 Pr4 Sb2 82.65(14) . 4_546
O4 Pr4 Sb2 86.4(2) 7_546 4_546
O4 Pr4 Sb2 150.7(2) 7_556 4_546
O2 Pr4 Sb2 85.23(15) 5_656 4_546
Sb2 Pr4 Sb2 67.0(2) 7_556 4_546
O5 Pr4 Sb2 83.00(13) . 4_556
O4 Pr4 Sb2 154.2(2) 7_546 4_556
O4 Pr4 Sb2 82.6(2) 7_556 4_556
O2 Pr4 Sb2 85.46(14) 5_656 4_556
Sb2 Pr4 Sb2 3.9(2) 7_556 4_556
Sb2 Pr4 Sb2 70.91(4) 4_546 4_556
O5 Pr4 Sb2 83.00(13) . 7_546
O4 Pr4 Sb2 82.58(19) 7_546 7_546
O4 Pr4 Sb2 154.2(2) 7_556 7_546
O2 Pr4 Sb2 85.46(14) 5_656 7_546
Sb2 Pr4 Sb2 70.91(3) 7_556 7_546
Sb2 Pr4 Sb2 3.9(2) 4_546 7_546
Sb2 Pr4 Sb2 74.8(2) 4_556 7_546
O5 Pr4 Ca5 37.2(7) . .
O4 Pr4 Ca5 101.5(4) 7_546 .
O4 Pr4 Ca5 101.5(4) 7_556 .
O2 Pr4 Ca5 128.3(7) 5_656 .
Sb2 Pr4 Ca5 53.1(5) 7_556 .
Sb2 Pr4 Ca5 53.1(5) 4_546 .
Sb2 Pr4 Ca5 55.2(5) 4_556 .
Sb2 Pr4 Ca5 55.2(5) 7_546 .
O5 Pr4 Ca2 147.57(13) . 7_556
O4 Pr4 Ca2 125.1(3) 7_546 7_556
O4 Pr4 Ca2 70.5(3) 7_556 7_556
O2 Pr4 Ca2 35.03(18) 5_656 7_556
Sb2 Pr4 Ca2 78.8(2) 7_556 7_556
Sb2 Pr4 Ca2 113.4(2) 4_546 7_556
Sb2 Pr4 Ca2 76.78(19) 4_556 7_556
Sb2 Pr4 Ca2 115.0(2) 7_546 7_556
Ca5 Pr4 Ca2 131.9(5) . 7_556
O5 Pr4 Ca2 147.57(13) . 7_546
O4 Pr4 Ca2 70.5(3) 7_546 7_546
O4 Pr4 Ca2 125.1(3) 7_556 7_546
O2 Pr4 Ca2 35.03(18) 5_656 7_546
Sb2 Pr4 Ca2 113.4(2) 7_556 7_546
Sb2 Pr4 Ca2 78.8(2) 4_546 7_546
Sb2 Pr4 Ca2 115.0(2) 4_556 7_546
Sb2 Pr4 Ca2 76.78(19) 7_546 7_546
Ca5 Pr4 Ca2 131.9(5) . 7_546
Ca2 Pr4 Ca2 64.9(3) 7_556 7_546
O5 Pr4 Pr5 36.06(8) . 7_546
O4 Pr4 Pr5 46.1(2) 7_546 7_546
O4 Pr4 Pr5 101.5(2) 7_556 7_546
O2 Pr4 Pr5 148.05(2) 5_656 7_546
Sb2 Pr4 Pr5 113.82(6) 7_556 7_546
Sb2 Pr4 Pr5 79.79(7) 4_546 7_546
Sb2 Pr4 Pr5 115.34(5) 4_556 7_546
Sb2 Pr4 Pr5 77.76(6) 7_546 7_546
Ca5 Pr4 Pr5 61.0(6) . 7_546
Ca2 Pr4 Pr5 165.2(2) 7_556 7_546
Ca2 Pr4 Pr5 113.69(15) 7_546 7_546
Pr5 Ca5 O5 108(4) . .
Pr5 Ca5 O5 62.5(19) . 7_546
O5 Ca5 O5 75.3(9) . 7_546
Pr5 Ca5 O5 62.5(19) . 7_556
O5 Ca5 O5 75.3(9) . 7_556
O5 Ca5 O5 103.1(17) 7_546 7_556
Pr5 Ca5 Sb2 138.6(19) . 7_556
O5 Ca5 Sb2 91.9(16) . 7_556
O5 Ca5 Sb2 159(2) 7_546 7_556
O5 Ca5 Sb2 89.6(5) 7_556 7_556
Pr5 Ca5 Sb2 138.6(19) . 4_546
O5 Ca5 Sb2 91.9(16) . 4_546
O5 Ca5 Sb2 89.6(5) 7_546 4_546
O5 Ca5 Sb2 159(2) 7_556 4_546
Sb2 Ca5 Sb2 73.7(13) 7_556 4_546
Pr5 Ca5 Sb2 135.1(17) . 4_556
O5 Ca5 Sb2 91.8(15) . 4_556
O5 Ca5 Sb2 162(2) 7_546 4_556
O5 Ca5 Sb2 85.6(5) 7_556 4_556
Sb2 Ca5 Sb2 4.1(2) 7_556 4_556
Sb2 Ca5 Sb2 77.8(13) 4_546 4_556
Pr5 Ca5 Sb2 135.1(17) . 7_546
O5 Ca5 Sb2 91.8(15) . 7_546
O5 Ca5 Sb2 85.6(5) 7_546 7_546
O5 Ca5 Sb2 162(2) 7_556 7_546
Sb2 Ca5 Sb2 77.8(13) 7_556 7_546
Sb2 Ca5 Sb2 4.1(2) 4_546 7_546
Sb2 Ca5 Sb2 81.9(13) 4_556 7_546
Pr5 Ca5 Pr4 148(4) . .
O5 Ca5 Pr4 40.4(10) . .
O5 Ca5 Pr4 100.1(11) 7_546 .
O5 Ca5 Pr4 100.1(11) 7_556 .
Sb2 Ca5 Pr4 60.4(10) 7_556 .
Sb2 Ca5 Pr4 60.4(10) 4_546 .
Sb2 Ca5 Pr4 62.2(9) 4_556 .
Sb2 Ca5 Pr4 62.2(9) 7_546 .
Pr5 Ca5 Sb2 68(3) . 8
O5 Ca5 Sb2 148.3(5) . 8
O5 Ca5 Sb2 123.2(18) 7_546 8
O5 Ca5 Sb2 75.3(8) 7_556 8
Sb2 Ca5 Sb2 76.2(6) 7_556 8
Sb2 Ca5 Sb2 112.1(11) 4_546 8
Sb2 Ca5 Sb2 74.3(5) 4_556 8
Sb2 Ca5 Sb2 113.6(11) 7_546 8
Pr4 Ca5 Sb2 136.5(12) . 8
Pr5 Ca5 Sb2 68(3) . 3_545
O5 Ca5 Sb2 148.3(5) . 3_545
O5 Ca5 Sb2 75.3(8) 7_546 3_545
O5 Ca5 Sb2 123.2(18) 7_556 3_545
Sb2 Ca5 Sb2 112.1(11) 7_556 3_545
Sb2 Ca5 Sb2 76.2(6) 4_546 3_545
Sb2 Ca5 Sb2 113.6(11) 4_556 3_545
Sb2 Ca5 Sb2 74.3(5) 7_546 3_545
Pr4 Ca5 Sb2 136.5(12) . 3_545
Sb2 Ca5 Sb2 61.6(7) 8 3_545
Pr5 Ca5 Pr5 91(3) . 7_546
O5 Ca5 Pr5 36.1(4) . 7_546
O5 Ca5 Pr5 40.2(5) 7_546 7_546
O5 Ca5 Pr5 94.3(11) 7_556 7_546
Sb2 Ca5 Pr5 123.0(15) 7_556 7_546
Sb2 Ca5 Pr5 84.3(7) 4_546 7_546
Sb2 Ca5 Pr5 124.2(15) 4_556 7_546
Sb2 Ca5 Pr5 81.9(7) 7_546 7_546
Pr4 Ca5 Pr5 62.9(7) . 7_546
Sb2 Ca5 Pr5 158.7(18) 8 7_546
Sb2 Ca5 Pr5 112.5(5) 3_545 7_546
Ca5 Pr5 O5 105.2(18) . 7_546
Ca5 Pr5 O5 105.2(18) . 7_556
O5 Pr5 O5 116.8(3) 7_546 7_556
Ca5 Pr5 O5 59(4) . .
O5 Pr5 O5 75.21(17) 7_546 .
O5 Pr5 O5 75.21(17) 7_556 .
Ca5 Pr5 O4 179(4) . .
O5 Pr5 O4 74.22(16) 7_546 .
O5 Pr5 O4 74.22(16) 7_556 .
O5 Pr5 O4 119.6(2) . .
Ca5 Pr5 Sb2 103(3) . 8
O5 Pr5 Sb2 139.81(18) 7_546 8
O5 Pr5 Sb2 81.27(18) 7_556 8
O5 Pr5 Sb2 144.66(12) . 8
O4 Pr5 Sb2 77.50(15) . 8
Ca5 Pr5 Sb2 103(3) . 3_545
O5 Pr5 Sb2 81.27(18) 7_546 3_545
O5 Pr5 Sb2 139.81(18) 7_556 3_545
O5 Pr5 Sb2 144.66(12) . 3_545
O4 Pr5 Sb2 77.50(15) . 3_545
Sb2 Pr5 Sb2 65.0(2) 8 3_545
Ca5 Pr5 Sb2 35.3(16) . 7_556
O5 Pr5 Sb2 140.49(17) 7_546 7_556
O5 Pr5 Sb2 82.96(17) 7_556 7_556
O5 Pr5 Sb2 78.00(13) . 7_556
O4 Pr5 Sb2 145.14(12) . 7_556
Sb2 Pr5 Sb2 73.21(11) 8 7_556
Sb2 Pr5 Sb2 105.97(11) 3_545 7_556
Ca5 Pr5 Sb2 35.3(16) . 4_546
O5 Pr5 Sb2 82.96(17) 7_546 4_546
O5 Pr5 Sb2 140.49(17) 7_556 4_546
O5 Pr5 Sb2 78.00(13) . 4_546
O4 Pr5 Sb2 145.14(12) . 4_546
Sb2 Pr5 Sb2 105.97(11) 8 4_546
Sb2 Pr5 Sb2 73.21(11) 3_545 4_546
Sb2 Pr5 Sb2 63.3(2) 7_556 4_546
Ca5 Pr5 Sb2 103(3) . 3
O5 Pr5 Sb2 142.90(17) 7_546 3
O5 Pr5 Sb2 77.68(18) 7_556 3
O5 Pr5 Sb2 141.14(11) . 3
O4 Pr5 Sb2 78.08(14) . 3
Sb2 Pr5 Sb2 3.9(2) 8 3
Sb2 Pr5 Sb2 68.90(3) 3_545 3
Sb2 Pr5 Sb2 71.46(4) 7_556 3
Sb2 Pr5 Sb2 107.75(3) 4_546 3
Ca5 Pr5 Sb2 103(3) . 8_545
O5 Pr5 Sb2 77.68(18) 7_546 8_545
O5 Pr5 Sb2 142.90(17) 7_556 8_545
O5 Pr5 Sb2 141.14(11) . 8_545
O4 Pr5 Sb2 78.08(14) . 8_545
Sb2 Pr5 Sb2 68.90(3) 8 8_545
Sb2 Pr5 Sb2 3.9(2) 3_545 8_545
Sb2 Pr5 Sb2 107.75(3) 7_556 8_545
Sb2 Pr5 Sb2 71.46(4) 4_546 8_545
Sb2 Pr5 Sb2 72.8(2) 3 8_545
Ca5 Pr5 Sb2 38.7(14) . 4_556
O5 Pr5 Sb2 143.60(17) 7_546 4_556
O5 Pr5 Sb2 79.38(17) 7_556 4_556
O5 Pr5 Sb2 78.53(12) . 4_556
O4 Pr5 Sb2 141.71(11) . 4_556
Sb2 Pr5 Sb2 71.42(3) 8 4_556
Sb2 Pr5 Sb2 107.79(3) 3_545 4_556
Sb2 Pr5 Sb2 3.8(2) 7_556 4_556
Sb2 Pr5 Sb2 67.14(3) 4_546 4_556
Sb2 Pr5 Sb2 69.47(11) 3 4_556
Sb2 Pr5 Sb2 109.77(11) 8_545 4_556
Pr2 Sb1 Pr2 180.00(5) 5 1_565
Pr2 Sb1 Pr2 72.97(4) 5 5_565
Pr2 Sb1 Pr2 107.03(4) 1_565 5_565
Pr2 Sb1 Pr2 107.03(4) 5 .
Pr2 Sb1 Pr2 72.97(4) 1_565 .
Pr2 Sb1 Pr2 180.00(3) 5_565 .
Pr2 Sb1 Pr1 110.85(3) 5 5_665
Pr2 Sb1 Pr1 69.15(3) 1_565 5_665
Pr2 Sb1 Pr1 69.73(4) 5_565 5_665
Pr2 Sb1 Pr1 110.27(4) . 5_665
Pr2 Sb1 Pr1 69.15(3) 5 1_455
Pr2 Sb1 Pr1 110.85(3) 1_565 1_455
Pr2 Sb1 Pr1 110.27(4) 5_565 1_455
Pr2 Sb1 Pr1 69.73(4) . 1_455
Pr1 Sb1 Pr1 180.00(5) 5_665 1_455
Pr2 Sb1 Pr1 69.73(4) 5 5_655
Pr2 Sb1 Pr1 110.27(4) 1_565 5_655
Pr2 Sb1 Pr1 110.85(3) 5_565 5_655
Pr2 Sb1 Pr1 69.15(3) . 5_655
Pr1 Sb1 Pr1 72.40(4) 5_665 5_655
Pr1 Sb1 Pr1 107.60(4) 1_455 5_655
Pr2 Sb1 Pr1 110.27(4) 5 1_465
Pr2 Sb1 Pr1 69.73(4) 1_565 1_465
Pr2 Sb1 Pr1 69.15(3) 5_565 1_465
Pr2 Sb1 Pr1 110.85(3) . 1_465
Pr1 Sb1 Pr1 107.60(4) 5_665 1_465
Pr1 Sb1 Pr1 72.40(4) 1_455 1_465
Pr1 Sb1 Pr1 180.00(5) 5_655 1_465
Pr2 Sb1 Ca1 72.83(19) 5 1_455
Pr2 Sb1 Ca1 107.17(19) 1_565 1_455
Pr2 Sb1 Ca1 111.1(2) 5_565 1_455
Pr2 Sb1 Ca1 68.9(2) . 1_455
Pr1 Sb1 Ca1 176.18(16) 5_665 1_455
Pr1 Sb1 Ca1 3.82(16) 1_455 1_455
Pr1 Sb1 Ca1 110.34(13) 5_655 1_455
Pr1 Sb1 Ca1 69.66(13) 1_465 1_455
Pr2 Sb1 Ca1 107.17(19) 5 5_665
Pr2 Sb1 Ca1 72.83(19) 1_565 5_665
Pr2 Sb1 Ca1 68.9(2) 5_565 5_665
Pr2 Sb1 Ca1 111.1(2) . 5_665
Pr1 Sb1 Ca1 3.82(16) 5_665 5_665
Pr1 Sb1 Ca1 176.18(16) 1_455 5_665
Pr1 Sb1 Ca1 69.66(13) 5_655 5_665
Pr1 Sb1 Ca1 110.34(13) 1_465 5_665
Ca1 Sb1 Ca1 180.0(4) 1_455 5_665
Pr2 Sb1 Ca1 68.9(2) 5 5_655
Pr2 Sb1 Ca1 111.1(2) 1_565 5_655
Pr2 Sb1 Ca1 107.17(19) 5_565 5_655
Pr2 Sb1 Ca1 72.83(19) . 5_655
Pr1 Sb1 Ca1 69.66(13) 5_665 5_655
Pr1 Sb1 Ca1 110.34(13) 1_455 5_655
Pr1 Sb1 Ca1 3.82(16) 5_655 5_655
Pr1 Sb1 Ca1 176.18(16) 1_465 5_655
Ca1 Sb1 Ca1 113.2(3) 1_455 5_655
Ca1 Sb1 Ca1 66.8(3) 5_665 5_655
Pr2 Sb1 Ca1 111.1(2) 5 1_465
Pr2 Sb1 Ca1 68.9(2) 1_565 1_465
Pr2 Sb1 Ca1 72.83(19) 5_565 1_465
Pr2 Sb1 Ca1 107.17(19) . 1_465
Pr1 Sb1 Ca1 110.34(13) 5_665 1_465
Pr1 Sb1 Ca1 69.66(13) 1_455 1_465
Pr1 Sb1 Ca1 176.18(16) 5_655 1_465
Pr1 Sb1 Ca1 3.82(16) 1_465 1_465
Ca1 Sb1 Ca1 66.8(3) 1_455 1_465
Ca1 Sb1 Ca1 113.2(3) 5_665 1_465
Ca1 Sb1 Ca1 180.0(4) 5_655 1_465
Ca5 Sb2 Ca5 77.8(13) 7_556 7_546
Ca5 Sb2 Pr3 108.6(7) 7_556 3_455
Ca5 Sb2 Pr3 171.2(8) 7_546 3_455
Ca5 Sb2 Pr4 66.4(8) 7_556 7_556
Ca5 Sb2 Pr4 107.3(6) 7_546 7_556
Pr3 Sb2 Pr4 70.91(11) 3_455 7_556
Ca5 Sb2 Pr5 74.2(6) 7_556 3_455
Ca5 Sb2 Pr5 113.6(8) 7_546 3_455
Pr3 Sb2 Pr5 74.59(12) 3_455 3_455
Pr4 Sb2 Pr5 114.0(2) 7_556 3_455
Ca5 Sb2 Pr3 174.1(7) 7_556 3_445
Ca5 Sb2 Pr3 100.6(7) 7_546 3_445
Pr3 Sb2 Pr3 72.44(4) 3_455 3_445
Pr4 Sb2 Pr3 108.99(5) 7_556 3_445
Pr5 Sb2 Pr3 111.55(4) 3_455 3_445
Ca5 Sb2 Pr4 107.4(6) 7_556 7_546
Ca5 Sb2 Pr4 62.6(8) 7_546 7_546
Pr3 Sb2 Pr4 109.02(5) 3_455 7_546
Pr4 Sb2 Pr4 70.91(4) 7_556 7_546
Pr5 Sb2 Pr4 174.9(2) 3_455 7_546
Pr3 Sb2 Pr4 66.99(11) 3_445 7_546
Ca5 Sb2 Pr5 6.1(7) 7_556 7_556
Ca5 Sb2 Pr5 72.7(7) 7_546 7_556
Pr3 Sb2 Pr5 114.0(2) 3_455 7_556
Pr4 Sb2 Pr5 71.55(11) 7_556 7_556
Pr5 Sb2 Pr5 74.03(11) 3_455 7_556
Pr3 Sb2 Pr5 172.8(2) 3_445 7_556
Pr4 Sb2 Pr5 107.05(4) 7_546 7_556
Ca5 Sb2 Ca3 112.0(7) 7_556 3_455
Ca5 Sb2 Ca3 169.2(8) 7_546 3_455
Pr3 Sb2 Ca3 3.69(19) 3_455 3_455
Pr4 Sb2 Ca3 74.0(3) 7_556 3_455
Pr5 Sb2 Ca3 74.6(3) 3_455 3_455
Pr3 Sb2 Ca3 69.23(16) 3_445 3_455
Pr4 Sb2 Ca3 108.7(3) 7_546 3_455
Pr5 Sb2 Ca3 117.3(3) 7_556 3_455
Ca5 Sb2 Pr5 113.8(8) 7_556 3_445
Ca5 Sb2 Pr5 69.9(6) 7_546 3_445
Pr3 Sb2 Pr5 111.65(4) 3_455 3_445
Pr4 Sb2 Pr5 176.8(2) 7_556 3_445
Pr5 Sb2 Pr5 68.90(3) 3_455 3_445
Pr3 Sb2 Pr5 70.51(11) 3_445 3_445
Pr4 Sb2 Pr5 106.2(2) 7_546 3_445
Pr5 Sb2 Pr5 108.54(4) 7_556 3_445
Ca3 Sb2 Pr5 108.5(3) 3_455 3_445
Ca5 Sb2 Ca5 67.9(11) 7_556 3_455
Ca5 Sb2 Ca5 105.7(5) 7_546 3_455
Pr3 Sb2 Ca5 82.7(8) 3_455 3_455
Pr4 Sb2 Ca5 114.8(4) 7_556 3_455
Pr5 Sb2 Ca5 8.7(9) 3_455 3_455
Pr3 Sb2 Ca5 118.0(7) 3_445 3_455
Pr4 Sb2 Ca5 168.3(8) 7_546 3_455
Pr5 Sb2 Ca5 67.1(7) 7_556 3_455
Ca3 Sb2 Ca5 82.9(8) 3_455 3_455
Pr5 Sb2 Ca5 67.8(3) 3_445 3_455
Ca5 Sb2 Pr5 72.4(6) 7_556 7_546
Ca5 Sb2 Pr5 6.2(7) 7_546 7_546
Pr3 Sb2 Pr5 176.82(10) 3_455 7_546
Pr4 Sb2 Pr5 107.13(4) 7_556 7_546
Pr5 Sb2 Pr5 108.58(3) 3_455 7_546
Pr3 Sb2 Pr5 106.2(2) 3_445 7_546
Pr4 Sb2 Pr5 67.83(11) 7_546 7_546
Pr5 Sb2 Pr5 67.14(3) 7_556 7_546
Ca3 Sb2 Pr5 175.3(3) 3_455 7_546
Pr5 Sb2 Pr5 70.23(11) 3_445 7_546
Ca5 Sb2 Pr5 100.5(8) 3_455 7_546
Ca2 O1 Ca1 107.4(4) . 3_455
Ca2 O1 Ca1 107.4(4) . 3_445
Ca1 O1 Ca1 122.5(8) 3_455 3_445
Ca2 O1 Pr2 11.1(4) . .
Ca1 O1 Pr2 111.5(4) 3_455 .
Ca1 O1 Pr2 111.5(4) 3_445 .
Ca2 O1 Pr1 115.3(2) . 3_455
Ca1 O1 Pr1 8.0(3) 3_455 3_455
Ca1 O1 Pr1 119.1(5) 3_445 3_455
Pr2 O1 Pr1 118.85(17) . 3_455
Ca2 O1 Pr1 115.3(2) . 3_445
Ca1 O1 Pr1 119.1(5) 3_455 3_445
Ca1 O1 Pr1 8.0(3) 3_445 3_445
Pr2 O1 Pr1 118.85(17) . 3_445
Pr1 O1 Pr1 114.7(3) 3_455 3_445
Ca2 O1 Pr1 114.7(5) . 5_655
Ca1 O1 Pr1 102.6(4) 3_455 5_655
Ca1 O1 Pr1 102.6(4) 3_445 5_655
Pr2 O1 Pr1 103.6(3) . 5_655
Pr1 O1 Pr1 97.0(2) 3_455 5_655
Pr1 O1 Pr1 97.0(2) 3_445 5_655
Ca2 O1 Ca1 120.4(7) . 5_655
Ca1 O1 Ca1 100.0(4) 3_455 5_655
Ca1 O1 Ca1 100.0(4) 3_445 5_655
Pr2 O1 Ca1 109.3(5) . 5_655
Pr1 O1 Ca1 93.9(2) 3_455 5_655
Pr1 O1 Ca1 93.9(2) 3_445 5_655
Pr1 O1 Ca1 5.7(3) 5_655 5_655
Ca2 O2 Ca2 126.1(7) 3_545 3
Ca2 O2 Pr2 11.3(4) 3_545 3_545
Ca2 O2 Pr2 121.9(4) 3 3_545
Ca2 O2 Pr2 121.9(4) 3_545 3
Ca2 O2 Pr2 11.3(4) 3 3
Pr2 O2 Pr2 115.6(3) 3_545 3
Ca2 O2 Pr4 107.4(4) 3_545 5_656
Ca2 O2 Pr4 107.4(4) 3 5_656
Pr2 O2 Pr4 117.97(17) 3_545 5_656
Pr2 O2 Pr4 117.97(17) 3 5_656
Ca2 O2 Ca4 103.4(6) 3_545 5_656
Ca2 O2 Ca4 103.4(6) 3 5_656
Pr2 O2 Ca4 114.5(3) 3_545 5_656
Pr2 O2 Ca4 114.5(3) 3 5_656
Pr4 O2 Ca4 10.5(8) 5_656 5_656
Ca2 O2 Pr3 105.0(4) 3_545 .
Ca2 O2 Pr3 105.0(4) 3 .
Pr2 O2 Pr3 97.7(2) 3_545 .
Pr2 O2 Pr3 97.7(2) 3 .
Pr4 O2 Pr3 103.8(2) 5_656 .
Ca4 O2 Pr3 114.3(8) 5_656 .
Ca2 O2 Ca3 102.1(5) 3_545 .
Ca2 O2 Ca3 102.1(5) 3 .
Pr2 O2 Ca3 93.8(3) 3_545 .
Pr2 O2 Ca3 93.8(3) 3 .
Pr4 O2 Ca3 111.1(5) 5_656 .
Ca4 O2 Ca3 121.6(9) 5_656 .
Pr3 O2 Ca3 7.3(4) . .
Ca3 O3 Ca3 125.8(9) 7_546 7_556
Ca3 O3 Ca1 108.5(5) 7_546 5_656
Ca3 O3 Ca1 108.5(5) 7_556 5_656
Ca3 O3 Pr1 111.1(5) 7_546 5_656
Ca3 O3 Pr1 111.1(5) 7_556 5_656
Ca1 O3 Pr1 7.9(4) 5_656 5_656
Ca3 O3 Pr3 8.7(4) 7_546 7_546
Ca3 O3 Pr3 120.3(5) 7_556 7_546
Ca1 O3 Pr3 117.2(2) 5_656 7_546
Pr1 O3 Pr3 119.58(17) 5_656 7_546
Ca3 O3 Pr3 120.3(5) 7_546 7_556
Ca3 O3 Pr3 8.7(4) 7_556 7_556
Ca1 O3 Pr3 117.2(2) 5_656 7_556
Pr1 O3 Pr3 119.58(17) 5_656 7_556
Pr3 O3 Pr3 114.0(3) 7_546 7_556
Ca3 O3 Pr2 101.0(5) 7_546 5_556
Ca3 O3 Pr2 101.0(5) 7_556 5_556
Ca1 O3 Pr2 111.0(5) 5_656 5_556
Pr1 O3 Pr2 103.1(3) 5_656 5_556
Pr3 O3 Pr2 96.5(2) 7_546 5_556
Pr3 O3 Pr2 96.5(2) 7_556 5_556
Ca3 O3 Ca2 97.7(6) 7_546 5_556
Ca3 O3 Ca2 97.7(6) 7_556 5_556
Ca1 O3 Ca2 118.6(6) 5_656 5_556
Pr1 O3 Ca2 110.7(4) 5_656 5_556
Pr3 O3 Ca2 92.3(3) 7_546 5_556
Pr3 O3 Ca2 92.3(3) 7_556 5_556
Pr2 O3 Ca2 7.6(3) 5_556 5_556
Ca4 O4 Ca4 133.7(15) 7_546 7_556
Ca4 O4 Ca3 105.1(9) 7_546 .
Ca4 O4 Ca3 105.1(9) 7_556 .
Ca4 O4 Pr3 107.7(9) 7_546 .
Ca4 O4 Pr3 107.7(9) 7_556 .
Ca3 O4 Pr3 9.2(4) . .
Ca4 O4 Pr4 10.5(9) 7_546 7_546
Ca4 O4 Pr4 125.1(9) 7_556 7_546
Ca3 O4 Pr4 115.3(3) . 7_546
Pr3 O4 Pr4 118.22(18) . 7_546
Ca4 O4 Pr4 125.1(9) 7_546 7_556
Ca4 O4 Pr4 10.5(9) 7_556 7_556
Ca3 O4 Pr4 115.3(3) . 7_556
Pr3 O4 Pr4 118.22(18) . 7_556
Pr4 O4 Pr4 115.8(4) 7_546 7_556
Ca4 O4 Pr5 98.8(8) 7_546 .
Ca4 O4 Pr5 98.8(8) 7_556 .
Ca3 O4 Pr5 115.6(6) . .
Pr3 O4 Pr5 106.4(3) . .
Pr4 O4 Pr5 95.7(2) 7_546 .
Pr4 O4 Pr5 95.7(2) 7_556 .
Ca5 O5 Pr5 110.5(6) . 7_546
Ca5 O5 Pr5 110.5(6) . 7_556
Pr5 O5 Pr5 116.8(3) 7_546 7_556
Ca5 O5 Pr4 102.4(15) . .
Pr5 O5 Pr4 107.79(16) 7_546 .
Pr5 O5 Pr4 107.79(16) 7_556 .
Ca5 O5 Pr5 12.8(15) . .
Pr5 O5 Pr5 104.79(17) 7_546 .
Pr5 O5 Pr5 104.79(17) 7_556 .
Pr4 O5 Pr5 115.1(3) . .
Ca5 O5 Ca4 112.9(16) . .
Pr5 O5 Ca4 102.9(4) 7_546 .
Pr5 O5 Ca4 102.9(4) 7_556 .
Pr4 O5 Ca4 10.6(7) . .
Pr5 O5 Ca4 125.7(8) . .
Ca5 O5 Ca5 104.7(9) . 7_546
Pr5 O5 Ca5 12.3(12) 7_546 7_546
Pr5 O5 Ca5 110.9(8) 7_556 7_546
Pr4 O5 Ca5 120.0(12) . 7_546
Pr5 O5 Ca5 97.0(10) . 7_546
Ca4 O5 Ca5 115.1(12) . 7_546
Ca5 O5 Ca5 104.7(9) . 7_556
Pr5 O5 Ca5 110.9(8) 7_546 7_556
Pr5 O5 Ca5 12.3(12) 7_556 7_556
Pr4 O5 Ca5 120.0(12) . 7_556
Pr5 O5 Ca5 97.0(10) . 7_556
Ca4 O5 Ca5 115.1(12) . 7_556
Ca5 O5 Ca5 103.1(18) 7_546 7_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ca1 O3 2.216(17) 5_656
Ca1 O1 2.238(9) 3_545
Ca1 O1 2.238(9) 3
Ca1 O1 2.670(15) 5_655
Ca1 Sb1 3.563(12) 1_655
Ca1 Sb1 3.563(12) 1_645
Ca1 Ca2 3.567(18) 3_545
Ca1 Ca2 3.567(18) 3
Ca1 Ca3 3.59(2) 3
Ca1 Ca3 3.59(2) 3_545
Ca1 Pr1 3.663(12) 7_645
Ca1 Pr1 3.663(12) 7_655
Pr1 O1 2.330(4) 3_545
Pr1 O1 2.330(4) 3
Pr1 O3 2.331(7) 5_656
Pr1 O1 2.454(7) 5_655
Pr1 Sb1 3.3211(14) 1_655
Pr1 Sb1 3.3211(14) 1_645
Pr1 Pr1 3.583(3) 7_645
Pr1 Pr1 3.583(3) 7_655
Pr1 Ca1 3.663(12) 7_645
Pr1 Ca1 3.663(12) 7_655
Pr1 Ca3 3.740(15) 3
Pr1 Ca3 3.740(15) 3_545
Ca2 O1 2.189(16) .
Ca2 O2 2.201(7) 3_455
Ca2 O2 2.201(7) 3_445
Ca2 O3 2.793(17) 5_556
Ca2 Ca1 3.567(18) 3_455
Ca2 Ca1 3.567(18) 3_445
Ca2 Ca4 3.64(3) 7_556
Ca2 Ca4 3.64(3) 7_546
Ca2 Sb1 3.639(13) 1_545
Ca2 Sb1 3.639(13) .
Ca2 Pr4 3.658(13) 7_556
Ca2 Pr4 3.658(13) 7_546
Pr2 O2 2.317(3) 3_455
Pr2 O2 2.317(3) 3_445
Pr2 O1 2.325(7) .
Pr2 O3 2.500(8) 5_556
Pr2 Sb1 3.2988(13) 1_545
Pr2 Sb1 3.2988(13) .
Pr2 Pr3 3.6101(14) 3_445
Pr2 Pr3 3.6101(14) 3_455
Pr2 Ca3 3.634(16) 3_445
Pr2 Ca3 3.634(16) 3_455
Pr2 Pr1 3.757(2) 5_655
Pr2 Ca1 3.772(13) 3_455
Ca3 O3 2.204(9) 7_546
Ca3 O3 2.204(9) 7_556
Ca3 O4 2.25(2) .
Ca3 O2 2.65(2) .
Ca3 Ca4 3.48(3) 7_546
Ca3 Ca4 3.48(3) 7_556
Ca3 Sb2 3.532(16) 8
Ca3 Sb2 3.532(16) 3_545
Ca3 Ca1 3.59(2) 3_445
Ca3 Ca1 3.59(2) 3_455
Ca3 Pr2 3.634(16) 3
Ca3 Pr2 3.634(16) 3_545
Pr3 O4 2.303(8) .
Pr3 O3 2.339(4) 7_546
Pr3 O3 2.339(4) 7_556
Pr3 O2 2.477(7) .
Pr3 Sb2 3.233(5) 8
Pr3 Sb2 3.233(5) 3_545
Pr3 Sb2 3.402(5) 3
Pr3 Sb2 3.402(5) 8_545
Pr3 Ca4 3.58(3) 7_546
Pr3 Ca4 3.58(3) 7_556
Pr3 Pr2 3.6101(14) 3
Pr3 Pr2 3.6101(14) 3_545
Ca4 O4 2.133(12) 7_546
Ca4 O4 2.133(12) 7_556
Ca4 O5 2.41(3) .
Ca4 O2 2.43(3) 5_656
Ca4 Ca3 3.48(3) 7_546
Ca4 Ca3 3.48(3) 7_556
Ca4 Pr3 3.58(3) 7_546
Ca4 Pr3 3.58(3) 7_556
Ca4 Ca2 3.64(3) 7_556
Ca4 Ca2 3.64(3) 7_546
Ca4 Sb2 3.68(3) 7_556
Ca4 Sb2 3.68(3) 4_546
Pr4 O5 2.307(6) .
Pr4 O4 2.315(4) 7_546
Pr4 O4 2.315(4) 7_556
Pr4 O2 2.336(6) 5_656
Pr4 Sb2 3.297(5) 7_556
Pr4 Sb2 3.297(4) 4_546
Pr4 Sb2 3.462(5) 4_556
Pr4 Sb2 3.462(5) 7_546
Pr4 Ca5 3.47(5) .
Pr4 Ca2 3.658(13) 7_556
Pr4 Ca2 3.658(13) 7_546
Pr4 Pr5 3.7245(14) 7_546
Ca5 Pr5 0.55(6) .
Ca5 O5 2.15(4) .
Ca5 O5 2.51(3) 7_546
Ca5 O5 2.51(3) 7_556
Ca5 Sb2 3.03(4) 7_556
Ca5 Sb2 3.03(4) 4_546
Ca5 Sb2 3.21(4) 4_556
Ca5 Sb2 3.21(4) 7_546
Ca5 Sb2 3.55(4) 8
Ca5 Sb2 3.55(4) 3_545
Ca5 Pr5 3.66(3) 7_546
Pr5 O5 2.303(3) 7_546
Pr5 O5 2.303(3) 7_556
Pr5 O5 2.379(6) .
Pr5 O4 2.698(9) .
Pr5 Sb2 3.385(5) 8
Pr5 Sb2 3.385(4) 3_545
Pr5 Sb2 3.466(4) 7_556
Pr5 Sb2 3.466(4) 4_546
Pr5 Sb2 3.546(5) 3
Pr5 Sb2 3.546(5) 8_545
Pr5 Sb2 3.624(5) 4_556
Sb1 Pr2 3.2988(13) 5
Sb1 Pr2 3.2988(13) 1_565
Sb1 Pr2 3.2988(13) 5_565
Sb1 Pr1 3.3211(13) 5_665
Sb1 Pr1 3.3211(13) 1_455
Sb1 Pr1 3.3211(13) 5_655
Sb1 Pr1 3.3211(13) 1_465
Sb1 Ca1 3.563(12) 1_455
Sb1 Ca1 3.563(12) 5_665
Sb1 Ca1 3.563(12) 5_655
Sb1 Ca1 3.563(12) 1_465
Sb2 Ca5 3.03(4) 7_556
Sb2 Ca5 3.21(4) 7_546
Sb2 Pr3 3.233(5) 3_455
Sb2 Pr4 3.297(4) 7_556
Sb2 Pr5 3.385(4) 3_455
Sb2 Pr3 3.402(5) 3_445
Sb2 Pr4 3.462(5) 7_546
Sb2 Pr5 3.466(4) 7_556
Sb2 Ca3 3.532(16) 3_455
Sb2 Pr5 3.546(5) 3_445
Sb2 Ca5 3.55(4) 3_455
Sb2 Pr5 3.624(5) 7_546
O1 Ca1 2.238(9) 3_455
O1 Ca1 2.238(9) 3_445
O1 Pr1 2.330(4) 3_455
O1 Pr1 2.330(4) 3_445
O1 Pr1 2.454(7) 5_655
O1 Ca1 2.670(15) 5_655
O2 Ca2 2.201(7) 3_545
O2 Ca2 2.201(7) 3
O2 Pr2 2.317(3) 3_545
O2 Pr2 2.317(3) 3
O2 Pr4 2.336(6) 5_656
O2 Ca4 2.43(3) 5_656
O3 Ca3 2.204(9) 7_546
O3 Ca3 2.204(9) 7_556
O3 Ca1 2.216(17) 5_656
O3 Pr1 2.331(7) 5_656
O3 Pr3 2.339(4) 7_546
O3 Pr3 2.339(4) 7_556
O3 Pr2 2.500(8) 5_556
O3 Ca2 2.793(17) 5_556
O4 Ca4 2.133(12) 7_546
O4 Ca4 2.133(12) 7_556
O4 Pr4 2.315(4) 7_546
O4 Pr4 2.315(4) 7_556
O5 Pr5 2.303(3) 7_546
O5 Pr5 2.303(3) 7_556
O5 Ca5 2.51(3) 7_546
O5 Ca5 2.51(3) 7_556
